- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Journal of Nanomaterials

Volume 2012 (2012), Article ID 387694, 7 pages

http://dx.doi.org/10.1155/2012/387694

## Synthesis of Bulk Nanostructured DO_{22} Superlattice of Ni_{3}(Mo, Nb) with High Strength, High Ductility, and High Thermal Stability

Center for Engineering Research, Research Institute, King Fahd University of Petroleum and Minerals, P.O. Box 1639, Dhahran 31261, Saudi Arabia

Received 8 May 2012; Accepted 2 June 2012

Academic Editor: Amir Kajbafvala

Copyright © 2012 H. M. Tawancy. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

We show that a bulk nanostructured material combining high strength, high ductility, and high thermal stability can be synthesized in a Ni-Mo-Nb alloy with composition approaching Ni_{3}(Mo, Nb). By means of a simple aging treatment at , the grains of the parent face-centered cubic phase are made to transform into nanosized ordered crystals with DO_{22} superlattice maintaining a size of 10–20 nm after up to 100 hours of aging and corresponding room-temperature yield strength of 820 MPa and tensile ductility of 35%. Deformation of the superlattice is found to predominantly occur by twinning on planes of the parent phase. It is concluded that, although the respective slip systems are suppressed, most of the twinning systems are preserved in the DO_{22} superlattice enhancing the ductility.

#### 1. Introduction

A common feature of bulk nanostructured materials [1–9] and intermetallic compounds [10] is relatively low ductility, which limits their usefulness as engineering materials. In the case of nanostructured materials, deformation behavior is more controlled by grain boundary migration and twinning as opposed to dislocation motion and multiplication. To improve ductility by promoting those deformation modes, research efforts have been focusing on synthesis techniques particularly severe plastic deformation [11–17]. Likewise, there has been an increasing interest in improving the ductility of intermetallic compounds and ordered alloys because of their unique combination of physical and chemical properties [18, 19].

Recently, it has been demonstrated that long-range ordering in Ni-Mo-based alloy can be used to synthesize bulk nanostructured superlattices combining high strength and high ductility [20–24]. It has been shown that the closely-related Pt_{2}Mo-type (Ni_{2}Mo), DO_{22} (Ni_{3}Mo), and (Ni_{4}Mo) superlattices coexist during long-range ordering in these systems [22, 23], which form the basis for many commercial alloys with important applications in the chemical process, petrochemical and power generation industries [25]. Each of these superlattices can directly be derived from the parent face-centered cubic structure by minor atoms rearrangement on planes. In the case of the Pt_{2}Mo-type superlattice, every third plane is occupied by Mo atoms and planes in-between contain only Ni atoms. Likewise, for the DO_{22} superlattice, every fourth plane is occupied by Mo atoms, and every fifth plane is occupied by Mo atoms in the case of the superlattice. Long-range ordering in these systems results in considerable strengthening corresponding to room-temperature yield strength of 800 MPa or higher [22]. However, the corresponding tensile ductility ranges from less than 5% to about 40% depending upon the exact chemical composition, which determines the most stable ordered phase and its morphology. Therefore, by balancing the chemical composition it is possible to synthesize bulk nanostructured superlattices with high strength and high ductility as demonstrated in the case of the superlattice of Ni_{4}Mo alloy [21, 22] and Ni-Mo-Cr alloys where the metastable Ni_{2}Mo with Pt_{2}Mo-type superlattice is stabilized by controlled amounts of Cr [23, 24]. In the case of binary Ni_{3}Mo alloy, large thin platelets of Ni_{3}Mo form during the earlier stages of thermal aging rendering the material extremely hard and brittle [26]. The objective of this paper is to show that bulk nanostructured DO_{22}-type superlattice with high strength, high ductility, and high thermal stability can be synthesized in a Ni-Mo-Nb alloy with a composition approaching Ni_{3}(Mo, Nb).

#### 2. Experimental Procedure

The alloy studied had a composition of 64.95 Ni-27.12 Mo-7.93 Nb in weight % corresponding to about 75.2 Ni-18.7 Mo-6.1 Nb in atomic %, approaching the Ni_{3}(Mo, Nb) composition. Sheets of the alloy about 1.5 mm in thickness were processed by standard techniques of vacuum induction melting, electroslag remelting, forging, hot rolling, and cold rolling. Metallographic specimens and tensile test specimens with 50.8 mm gage length were given recrystallization anneal at 1065°C for 15 minutes followed by water quenching. Specimens for light optical metallography were etched in a solution consisting of 80% HCl and 20% of 15 mol % chromic acid to reveal the initial grain structure. Thermal aging experiments were carried out at 700°C for up to 100 hours followed by air cooling. All tensile tests were conducted at room temperature and the fracture surfaces were examined in the secondary electron mode of a scanning electron microscope operating at 20 keV. Thin foils for transmission electron microscopy were prepared by the jet polishing technique in a solution of 30% nitric acid in methanol. All the foils were examined at an accelerating voltage of 200 keV. Since the parent fcc structure and DO_{22} superlattice are closely related, all diffraction patterns are indexed in terms of the fcc structure.

#### 3. Results and Discussion

Figure 1 summarizes characteristic structural features of the alloy studied in the annealed condition. The gross grain structure is shown in the light optical micrograph of Figure 1(a). Full recrystallization is indicated by the high density of annealing twins, which typifies an fcc material with relatively low stacking fault energy [27]. Similar to the case of binary Ni-Mo alloys, the alloy contained short-range order as indicated by the appearance of diffuse intensity maxima at positions in the <100> electron diffraction pattern of Figure 1(b). It has been reported in an earlier study that short-range order tends to lower the stacking fault energy [28]. This is found to be consistent with the observed deformation substructure. As an example, Figure 1(c) is a bright-field TEM image showing the deformation substructure corresponding to 10% tensile elongation at room temperature. Visible slip lines (traces of planes) and the relatively low tendency for dislocation to cross slip are common features of fcc materials having relatively low stacking fault energy [27]. This has an important implication on the preferred deformation mode in the ordered state, which enhances ductility as shown later.

During the early stages of thermal aging (15 minutes at 700°C) very fine precipitates were observed as shown in the example of Figure 2. The bright-field TEM image of Figure 2(a) shows that the precipitates assume the morphology of thin short platelets revealed by elastic strain contrast. At this stage, the precipitates appeared to be too fine to produce characteristic diffraction effects. Figure 2(b) is a one-dimensional lattice image of planes showing a highly coherent precipitate with a thickness of about 1.5 nm. However, with continued thermal exposure, characteristic reflections of the DO_{22} superlattice at , , and positions were observed as demonstrated in Figure 3. A schematic illustration of the crystallographic relationship between the parent fcc lattice and DO_{22} superlattice is given in Figure 3(a). The corresponding reciprocal lattice intersection is shown in Figure 3(b), which is to be compared with the observed <100> diffraction pattern of Figure 3(c) obtained after 24 hours of aging at 700°C. As can be seen, the observed diffraction pattern contains the characteristic reflections of the DO_{22} superlattice. Figures 3(d) and 3(e) show corresponding diffraction patterns in <110> and <112> orientations, respectively, where only reflections can be present in the <110> pattern, and the <112> pattern can contain both the , and superlattice reflections.

Figure 4 shows dark-field TEM images illustrating the ordered microstructure of one crystallographic variant of the DO_{22} superlattice. Both images were formed with superlattice reflections as illustrated in the inset of Figure 4(a). It is observed that the superlattice assumes the morphology of nanosized particles with an average size of 10–20 nm. Also, it is observed as the aging time was extended from 24 hours (Figure 4(a)) to 100 hours (Figure 4(b)), the change in superlattice morphology was insignificant demonstrating its relatively high thermal stability. The corresponding effect of short-range order → long-range order transformation on the room temperature tensile properties is summarized in Figure 5. After 1 hour of aging at 700°C, the 0.2% yield strength was nearly doubled reaching about 800 MPa. However, the material retained about 80% of its initial ductility in the short-range ordered state. With continued aging up to 100 hours, the material maintained a combination of high yield strength of about 820 MPa and high tensile ductility of about 35% consistent with the observed high thermal stability of the DO_{22} superlattice.

Comparative true tensile stress-strain diagrams in the short-range and long-range ordered states are shown in Figure 6. It is noted that the strain hardening rate is significantly lowered by long-range ordering to the DO_{22} superlattice reflecting a change in the deformation behavior. In contrast with the short-range ordered state where deformation behavior typifies an fcc material with relatively low stacking fault energy as demonstrated in Figure 1(c), twinning on planes is found to be the predominant deformation mode in the long-range ordered state as illustrated in the example of Figure 7. This indicates that although long-range ordering could suppress most of the slip systems characteristic of the parent fcc lattice, many of the twinning systems remain active suggesting that the stacking fault energy of the material is further lowered by long-range ordering enhancing deformation by twinning. A similar behavior is found to occur in ordered Ni-Mo [21, 22] and Ni-Mo-Cr [23, 24] alloys.

Figure 8 shows secondary electron SEM images illustrating the morphology of tensile fractures surfaces in the annealed (short-range ordered) and aged (long-range ordered) states. Typical of ductile materials, in both cases, fracture occurred by dimple-type rupture. However, in the long-range ordered state, the dimples can be seen to be finer and shallower, which could be related to higher density of crack nucleation sites as well as relatively lower ductility in the long-range ordered state.

#### 4. Conclusion

It is concluded that a bulk nanostructured DO_{22} superlattice with high strength, high ductility, and high thermal stability can be synthesized in a Ni-Mo-Nb alloy with composition approaching Ni_{3}(Mo, Nb) by a simple aging heat treatment at 700°C. Upon thermal aging, the grains of the high-temperature fcc phase are subdivided into ordered crystals on the nanoscale (10–20 nm) with room-temperature yield strength of about 820 MPa and tensile ductility of 35%. Plastic deformation in the ordered state is found to predominantly occur by twinning on planes of the parent fcc structure indicating that the superlattice preserves the twinning systems of the parent phase leading to the observed high ductility.

#### Acknowledgment

It is a pleasure to acknowledge the continued support of King Fahd University of Petroleum and Minerals.

#### References

- Y. Zhao and X. Liao, “Ductility of bulk nanostructured materials,” in
*Materials Science Forum*, vol. 633-634, Trans Technical, Zurich, Switzerland, 2010. View at Google Scholar - C. C. Koch, “Nanostructured materials: an overview,” in
*Bulk Nanostructured Materials*, M. J. Zehetbauer and Y. T. Zhu, Eds., pp. 1–20, Wiley-VCH, Weinheim Germany, 2009. View at Google Scholar - E. Bitzek, C. Brandl, P. M. Derlet, and H. Van Swygenhoven, “Dislocation cross-slip in nanocrystalline fcc metals,”
*Physical Review Letters*, vol. 100, no. 23, Article ID 235501, 4 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - H. Van Swygenhoven and J. R. Weertman, “Deformation in nanocrystalline metals,”
*Materials Today*, vol. 9, no. 5, pp. 24–31, 2006. View at Publisher · View at Google Scholar · View at Scopus - Y. T. Zhu and X. Liao, “Nanostructured metals: retaining ductility,”
*Nature Materials*, vol. 3, no. 6, pp. 351–352, 2004. View at Publisher · View at Google Scholar · View at Scopus - Z. Budrovic, H. Van Swygenhoven, P. M. Derlet, S. Van Petegem, and B. Schmitt, “Plastic deformation with reversible peak broadening in nanocrystalline nickel,”
*Science*, vol. 304, no. 5668, pp. 273–276, 2004. View at Publisher · View at Google Scholar · View at Scopus - C. C. Koch, “Optimization of strength and ductility in nanocrystalline and ultrafine grained metals,”
*Scripta Materialia*, vol. 49, no. 7, pp. 657–662, 2003. View at Publisher · View at Google Scholar · View at Scopus - H. Van Swygenhoven and J. R. Weertman, “Preface to the viewpoint set on: mechanical properties of fully dense nanocrystalline metals,”
*Scripta Materialia*, vol. 49, no. 7, pp. 625–627, 2003. View at Publisher · View at Google Scholar · View at Scopus - D. Jia, Y. M. Wang, K. T. Ramesh, E. Ma, Y. T. Zhu, and R. Z. Valiev, “Deformation behavior and plastic instabilities of ultrafine-grained titanium,”
*Applied Physics Letters*, vol. 79, no. 5, pp. 611–613, 2001. View at Publisher · View at Google Scholar · View at Scopus - R. W. Cahn, “Intermetallics: new physics,”
*Contemporary Physics*, vol. 42, no. 6, pp. 365–375, 2001. View at Publisher · View at Google Scholar · View at Scopus - P. Xue, B. L. Xiao, and Z. Y. Ma, “High tensile ductility via enhanced strain hardening in ultrafine-grained Cu,”
*Materials Science and Engineering A*, vol. 532, pp. 106–110, 2012. View at Publisher · View at Google Scholar · View at Scopus - D. G. Morris and M. A. Munoz-Morris, “Microstructural refinement in alloys and intermetallics by severe plastic deformation,”
*Journal of Alloys and Compounds*. In press. View at Publisher · View at Google Scholar - K. V. León, M. A. Muñoz-Morris, and D. G. Morris, “Optimisation of strength and ductility of Cu-Cr-Zr by combining severe plastic deformation and precipitation,”
*Materials Science and Engineering A*, vol. 536, pp. 181–189, 2012. View at Publisher · View at Google Scholar · View at Scopus - Y. Zhao, Y. Zhu, and E. J. Lavernia, “Strategies for improving tensile ductility of bulk nanostructured materials,”
*Advanced Engineering Materials*, vol. 12, no. 8, pp. 769–778, 2010. View at Publisher · View at Google Scholar · View at Scopus - M. A. Muñoz-Morris and D. G. Morris, “Severe plastic deformation processing of Al-Cu-Li alloy for enhancing strength while maintaining ductility,”
*Scripta Materialia*, vol. 63, no. 3, pp. 304–307, 2010. View at Publisher · View at Google Scholar · View at Scopus - Y. Zhao, T. Topping, J. F. Bingert et al., “High tensile ductility and strength in bulk nanostructured nickel,”
*Advanced Materials*, vol. 20, no. 16, pp. 3028–3033, 2008. View at Publisher · View at Google Scholar · View at Scopus - R. Z. Valiev, “The new trends in fabrication of bulk nanostructured materials by SPD processing,”
*Journal of Materials Science*, vol. 42, no. 5, pp. 1483–1490, 2007. View at Publisher · View at Google Scholar · View at Scopus - K. A. Gschneidner, M. Ji, C. Z. Wang et al., “Influence of the electronic structure on the ductile behavior of B2 CsCl-type AB intermetallics,”
*Acta Materialia*, vol. 57, no. 19, pp. 5876–5881, 2009. View at Publisher · View at Google Scholar · View at Scopus - K. Gschneidner, A. Russell, A. Pecharsky et al., “A family of ductile intermetallic compounds,”
*Nature Materials*, vol. 2, no. 9, pp. 587–590, 2003. View at Publisher · View at Google Scholar · View at Scopus - H. M. Tawancy, “Corrosion resistant Nickel-Base Alloys,” US Patent no. 7, 922, 969, 2011.
- H. M. Tawancy and M. O. Aboelfotoh, “Yttrium-doped nanocrystalline Ni
_{4}Mo: ultrahigh strength and high ductility combined with useful intermetallic properties,”*Journal of Materials Science*, vol. 45, no. 13, pp. 3413–3418, 2010. View at Publisher · View at Google Scholar · View at Scopus - H. M. Tawancy, “Long-range ordering: an approach to synthesize nanoscale Ni-Mo-based superlattices with high strength and high ductility,”
*Materials Science Forum*, vol. 633-634, pp. 421–435, 2010. View at Publisher · View at Google Scholar · View at Scopus - H. M. Tawancy and M. O. Aboelfotoh, “Application of long-range ordering in the synthesis of a nanoscale Ni
_{2}(Cr,Mo) superlattice with high strength and high ductility,”*Materials Science and Engineering A*, vol. 500, no. 1-2, pp. 188–195, 2009. View at Publisher · View at Google Scholar · View at Scopus - H. M. Tawancy and M. O. Aboelfotoh, “High strength and high ductility in a nanoscale superlattice of Ni
_{2}(Cr,Mo) deformable by twinning,”*Scripta Materialia*, vol. 59, no. 8, pp. 846–849, 2008. View at Publisher · View at Google Scholar · View at Scopus - F. G. Hodge, “Nickel and high-nickel alloys,” in
*Corrosion and Corrosion Protection Handbook*, P. A. Schweitzer, Ed., pp. 65–69, Marcel-Dekker, New York, NY, USA, 1983. View at Google Scholar - H. M. Tawancy, “Long-range ordering behaviour and mechanical properties of Ni-Mo-based alloys,”
*Journal of Materials Science*, vol. 30, no. 2, pp. 522–537, 1995. View at Publisher · View at Google Scholar · View at Scopus - P. R. Swann, “Dislocation arrangements in face-centered cubic materials,” in
*Electron Microscopy and Strength and Crystals*, G. Thomas and J. Washburn, Eds., pp. 131–181, Wiley Interscience, New York, NY, USA, 1963. View at Google Scholar - P. R. Okamoto and G. Thomas, “On short range order and micro-domains in the Ni
_{4}Mo system,”*Acta Metallurgica*, vol. 19, no. 8, pp. 825–841, 1971. View at Google Scholar · View at Scopus